Graphite as radioactive waste: corrosion behaviour
under final repository conditions and thermal
Von der Fakultät für Georessourcen und Materialtechnik der
Rheinisch-Westfälischen Technischen Hochschule Aachen
zur Erlangung des akademischen Grades eines
Doktors der Naturwissenschaften
vorgelegt von Magister Chemiker
aus Novosibirsk, Rußland
Berichter: Univ.-Prof. Dr. rer. nat. Reinhard Odoj
Prof. Dr. Horst Pentinghaus
Graphite as radioactive waste: corrosion behaviour under final repository conditions and thermal treatment
The present work deals with radioactive graphite management. Two different aspects were examined:
1. The corrosion behaviour of graphite under final repository conditions 2. The decontamination of graphite by thermal treatment
Spent fuel from the German AVR and THTR high-temperature reactors is envisaged for direct disposal in a final repository. In this respect, corrosion of the graphite matrix of the spherical fuel elements and pyrocarbon coatings from coated fuel particles is a very important aspect for predicting the long-term behaviour of the radioactive waste.
The graphite materials to be examined were isolated from unirradiated fuel elements, and their corrosion was investigated in different aqueous phases. The experiments were performed
in deionised water, MgCl2-rich (brine-2) and NaCl-rich (brine-3) solutions at 90°C under
argon, oxygen and air atmosphere. In order to investigate the influence of aqueous phase radiolysis, further experiments were performed in the presence of J-irradiation sources under argon atmosphere.
It was established that the slow corrosion of carbonaceous materials in different aquatic phases in the absence of irradiation was caused by interaction with dissolved oxygen. Corrosion rates in aqueous solutions under pure oxygen and air atmosphere decrease in the order water > brine-3 > brine-2. Acceleration of graphite and pyrocarbon corrosion was observed in the presence of J-irradiation in brines while the opposite influence of the aqueous phases on the corrosion rates was additionally observed. The corrosion rates of graphite and pyrocarbon in irradiated brine-2 and brine-3 in argon atmosphere were two orders of magnitude higher than in pure oxygen atmosphere without irradiation. This may be related to the formation of highly oxidising chlorine species in brines, which react with carbon materials. In pure water, radiolysis did not influence the oxidation process significantly. However, calculating the expected lifetime of the graphite matrix in the repository on the basis of the corrosion rates determined is an extremely conservative consideration since the radiation dose rates used are significantly higher than could ever occur during final disposal of high-temperature reactor fuel elements.
In the second part of the present work, thermal treatment of contaminated structural graphite from the high-temperature reactor core and thermal columns of the research reactors was investigated as a possible decontamination process. The main problem associated with direct disposal of contaminated graphite is its large volume. Reprocessing of the graphite based on graphite gasification offers the opportunity to separate the radionuclides from the main graphite mass, which could then be reused or disposed conventionally.
The experiments were performed in an argon flow and steam in the temperature range of
870 – 1060°C. Comparison of the release rate ratios of the volatilised radionuclides 14C and
3H with the release of 12C showed that under all experimental conditions tritium and 14C were
released faster than the graphite sample was oxidised.
The maximum value of the release rate ratio was obtained for tritium in experiments with argon atmosphere at 1060°C.
separation of carbon isotopes is only possible because 14C is mainly located near the grain
boundary surfaces and its concentration profile decreases with depth inside the graphite grains.
The radionuclides 60Co, 154,155Eu, 134,137Cs and 133Ba present in contaminated graphite mainly
remained in the ceramic reaction boat in contrast to the volatile Cs.
By optimising the process parameters this decontamination process may be developed further
into a pilot scale technology for graphite purification with fractional reduction of the 14C
Graphit als radioaktiver Abfall: Korrosionsverhalten unter Endlagerbedingungen und thermische Behandlung
Diese Arbeit steht im Zusammenhang mit der Entsorgung von radioaktivem Graphit. Dabei wurden zwei verschiedene Aspekte betrachtet:
1. Das Korrosionsverhalten von Graphit unter Endlagerbedingungen 2. Die Dekontamination von Graphit durch eine thermische Behandlung
Da die beim Betrieb der deutschen Hochtemperaturreaktoren AVR und THTR angefallen Brennelemente direkt endgelagert werden sollen, ist die Korrosion der Graphit-Matrix der kugelförmigen Brennelemente und Pyrokohlenstoffschichten der Brennstoffpartikel von großer Bedeutung für die Vorhersage des Langzeitverhaltens dieser Abfälle.
Die Graphitmaterialien wurden aus unbestrahlten Brennelementen isoliert und deren Korrosion in verschiedenen wässrigen Phasen untersucht. Die Versuche wurden in
destilliertem Wasser sowie in MgCl2-reichen (Lauge-2) und NaCl-reichen (Lauge-3)
Lösungen bei 90°C in Gegenwart von Argon, Sauerstoff und Luftatmosphäre durchgeführt. Um den Einfluss der Radiolyse der wässrigen Phase zu untersuchen, wurden weitere Experimente unter Argon-Atmosphäre mit äußerer J-Bestrahlung durchgeführt.
Es wurde festgestellt, dass eine langsame Korrosion der kohlenstoffhaltigen Materialien in verschiedenen Lösungen ohne Bestrahlung durch die Wechselwirkung mit gelöstem Sauerstoff auftritt. Die Korrosionsraten in wässrigen Lösungen in Gegenwart einer reinem Sauerstoffatmosphäre und Luftatmosphäre nehmen in der Reihenfolge Wasser> Lauge-3> Lauge-2 ab. Unter dem Einfluss von J-Strahlung wurde eine beschleunigte Korrosion beobachtet, wobei zusätzlich ein entgegengesetzter Einfluss der wässrigen Phasen auf die Korrosionsraten beobachtet wurde. Die Korrosionsraten des Graphits und Pyrokohlenstoffs in bestrahlter Lauge-2 und Lauge-3 in der Argon-Atmosphäre waren zwei Größenordnungen höher als in der reinen Sauerstoff-Atmosphäre ohne Bestrahlung. Dies ist mit Bildung von reaktiven, oxidierenden Chlor-Spezies in den Salzlaugen verbunden, die dann mit Kohlenstoff-Materialien reagieren. In reinem Wasser beeinflusste die Radiolyse den Oxydationsprozess nicht signifikant. Die Berechnung der im Endlager zu erwartenden Lebensdauer der Graphitmatrix auf Grund der ermittelten Korrosionsraten ist jedoch eine extrem konservative Betrachtung, da die verwendeten Strahlungsdosisraten wesentlich höher waren, als sie bei der Endlagerung der Hochtemperaturreaktorbrennelemente jemals auftreten könnten.
Im zweiten Teil der Arbeit wurde die thermische Behandlung von kontaminiertem Strukturgraphit aus dem Core der Hochtemperaturreaktoren und thermischen Säulen aus Forschungsreaktoren als mögliches Dekontaminationsverfahren untersucht. Das mit der direkten Endlagerung des kontaminierten Graphits verbundene Hauptproblem ist sein großes Volumen. Die Aufbereitung des Graphits, basierend auf der Graphit-Vergasung, bietet die Möglichkeit, die Radionuklide vom inaktiven Kohlenstoff zu trennen, der dann weiter verwendet oder konventionell entsorgt werden könnte.
Die Untersuchungen wurden in Argon- und Wasserdampf-Atmosphäre in einem Temperaturbereich von 870 - 1060°C durchgeführt. Der Vergleich der Verhältnisse der
Freisetzungsraten von 14C und 3H zu 12C zeigte, dass bei allen experimentellen Bedingungen
Des weiteren konnte gezeigt werden, dass 14C mit Anreicherungsfaktoren von bis zu 20
gegenüber 12C von der Hauptmenge des Graphits abgetrennt werden kann. Jedoch ist der
Gesamtumsatz unter diesen Bedingungen nicht ausreichend für einen technischen Prozess. Durch Zusatz von Wasserdampf kann der Gesamtumsatz erhöht werden, wobei die Anreichungsfaktoren jedoch auf unter 5 absinken. Generell ist diese Trennung der
Kohlenstoffisotope nur deshalb möglich, weil sich das 14C hauptsächlich nahe der
Korngrenzenoberflächen befindet und sein Konzentrationsprofil mit der Tiefe innerhalb der Graphitkörner abnimmt.
Die Radionuklide 60Co, 154,155Eu, 134,137Cs und 133Ba, die im radioaktiven Graphit gegenwärtig
sind, verblieben während der thermischen Behandlung, mit Ausnahme des flüchtigeren Cs, hauptsächlich in dem verwendeten Keramikreaktionsgefäß.
Durch eine weitere Optimierung der Verfahrensparameter könnte diese Methode zu einem
technischem Verfahren zur Reinigung von Graphit mit einer partiellen Reduktion des 14
A. Introduction and objectives ...1
B. Statement of problem...3
B.1. Graphite in nuclear technology ...3
B.1.1. Graphite structure...3
B.1.2. Chemical reactions of carbon...4
B.1.2.1. Gas-phase reactions...4
B.1.2.2. Liquid-phase reactions...6
B.1.3. Graphite in reactor core structure ...7
B.1.3.1. Design of AVR core structure ...7
B.1.3.2. Nuclear graphite manufacture ...8
B.1.4. Graphite fuel elements...9
B.1.5. Pyrolitic carbon coatings for fuel particles...9
B.1.6. Fabrication method of graphite matrix...12
B.2. Graphite waste management ...14
B.2.1. Nature of radionuclide contamination...14
B.2.2. Diffusion of radionuclides in graphite...16
B.2.3. Options of graphite waste management...19
B.2.4. Reprocessing of contaminated graphite...20
B.2.5. Deep geological disposal ...22
B.2.5.1. Host rock types...22
B.2.5.2. Multi-barrier system...22
B.2.5.3. Water radiolysis in repository...23
C. Experimental part ...27
C.1. Equipment ...27
C.2. Reagents and materials investigated...28
C.3. Performance of experiments...29
C.3.1. Graphite oxidation ...29
C.3.1.1. Sample preparation...29
C.3.1.2. Oxidation experiments without irradiation...29
C.4. Characterisation of graphite and pyrocarbon materials ...37
D. Results and discussion ...41
D.1. Graphite corrosion in aqueous phase ...41
D.1.1. Oxidation without J-irradiation ...41
D.1.2. Graphite oxidation with hydrogen peroxide...42
D.1.3. Graphite and pyrocarbon oxidation in the presence of J-irradiation field...44
D.1.4. The lifetime estimation of pyrocarbon coatings and graphite protective layer...49
D.2. Graphite treatment...54
D.2.1. Treatment in argon atmosphere...54
D.2.1.1. Tritium release...54
D.2.2. Oxidation with water steam...56
D.2.2.1. Tritium release...56
D.2.3. Release rates ...60
D.2.3.1. Release rates under inert atmosphere ...61
D.2.3.2. Release rates under oxidising conditions ...66
D.2.3.3. Comparison of treatment regimes ...68
D.2.4. Migration of other radionuclides during graphite thermal treatment...70
E. Summary and outlook...73
H.1. List of tables ...110
A. Introduction and objectives
Graphite has been widely used as a moderator, reflector and fuel matrix in various types of nuclear reactors. At the end of the reactor’s life activated graphite and carbon installations are radioactive waste, which requires a special waste management strategy.
In Germany two high temperature gas-cooled and graphite moderated reactors were developed: the 15 MWe AVR (Arbeitsgemeinschaft Versuchsreaktor) plant and the 300 MWe Thorium High Temperature Reactor (THTR 300). At the end of 1988 the reactors were shut down (AVR after 21 years of operating and THTR after 3 years of operating). About 300000 AVR and 620 000 THTR fuel elements were irradiated during the operational time. The fuel of this reactor type consists of small uranium/thorium oxide spherical particles of about 0.5 mm in size. The fuel particles are coated with pyrocarbon coating (BISO) or a combination of pyrocarbon and silicon carbide coatings (TRISO) up to 1 mm in total diameter. About 20000 coated particles are embedded in a graphite matrix of spherical form about 6 cm in diameter. The proposed solution for HTR spent fuel management in Germany is storage in deep geological formations without reprocessing. Three types of rocks are considered as host units: granite, clay and salt domes. The long term safety depends on the integrity of the multibarrier system of the waste package  and the integrity of spent fuel element itself.
As an accident scenario ground water ingress into the repository and its interaction with the protective barriers of graphite and the pyrocarbon coatings should be taken into account. The first experiments with HTR spent fuel elements demonstrated that extremely low amounts of radionuclides were released from the graphite matrix and coated particles . However, the chemical impact of aqueous phases on graphite matrix and pyrocarbon coatings in the long term is unknown. In this respect, the investigation of graphite and pyrocarbon behaviour in repository relevant conditions is important.
The other problem is associated with reflector graphite, which becomes a radioactive waste at the end of reactor life. Direct disposal in deep geological formations is one of the most probable ways of radioactive graphite management. However, the large volume of contaminated graphite significantly reduces the cost efficiency of this management route. For example, in the case of AVR decommissioning 67 Mg of reflector graphite and 158 Mg of carbon isolation represent a great volume of low and medium active radioactive waste. This graphite contains significant quantities of radionuclides from the neutron activation of impurities and contamination with fission products. Reprocessing of the graphite offers the opportunity to separate the majority of the short-lived isotopes from the graphite. Thereafter only a small active residue fraction has to be disposed and the main mass of graphite can be reused.
The existing purification procedure is based on graphite gasification. This procedure allows
non-volatile and volatile radionuclides to be separated by chemical methods. The CO2formed
can be released to the atmosphere or precipitated as carbonates. Chemical methods are not
capable of separating the carbon isotopes: long-lived radioactive 14C and non-radioactive 12C.
In principle, the off-gases from incineration can be fractionated in order to recover 14C by
isotope separation. However, the development of a more simple method for graphite
purification from 14C would give an additional economical benefit.
x Investigation of the influence of high-temperature treatment on the release of radioactive carbon and other radionuclides from contaminated graphite.
B. Statement of problem
B.1. Graphite in nuclear technology
The properties of graphite make it suitable for many nuclear applications. By far the greatest use has been as a moderator and reflector, because nuclear graphite has an absorption cross section for thermal neutrons as low as 3.5 to 3.8 mb. Furthermore, graphite is strong enough to serve as a structural component, eliminating the necessity of using metals with higher cross sections.
The high-temperature strength, stability, and thermal conductivity of graphite make it good for use in high-temperature reactors as a matrix material for ceramic fuels such as the uranium oxides and carbides.
In the reactor core, boronated graphite is sometimes used as a high-temperature control-rod material. Designs for gas-cooled reactors employ graphite sleeves that support the fuel elements and channel the coolant. Also it is useful as a container for reactor irradiation experiments.
B.1.1. Graphite structure
Pure graphite is one of the most chemically inert materials. It is resistant to most acids, alkalis and corrosive gases. The crystallographic structure has a considerable influence on the chemical reactivity of graphite.
The basis of the crystal structure of graphite is the graphene plane of the carbon layer plane,
i.e. an extended hexagonal array of carbon atoms with sp2 V bonding and delocalised S
bonding. The most common crystal form of graphite is hexagonal and consists of a stack of layer planes in the stacking sequence ABABAB
The rhombohedral form of graphite with a stacking sequence ABCABC is a minor component
of well-crystallised graphite. The theoretical density of both forms of graphite is 2.26 g/cm3;
the in-plane C–C distance is 0.142 nm and the interlayer distance 0.335 nm. Such a difference results from different types of chemical bonding. The usual assumption is that interlayer potentials are of van der Waals type. The bond strength within the layer planes is approximately 150 kcal/(gram atom), whereas the interlayer binding energy is estimated to be 1.3 kcal/(gram atom).
The structure given in Figure 1 is the perfect crystal structure of graphite. Solid carbons, in general, are less perfect. They consist of domains of carbon atoms arranged in a hexagonal pattern but these domains vary in degree of ordering and value of interlayer space. Interlayer spacing is larger than for the graphite crystal (up to 0.344 instead of 0.335nm). The most disordered carbons have a so-called “turbostratic” structure with carbon layer planes oriented randomly about the c-axis.
Pyrolitic carbon has such a structure, usually with many warped basal planes, lattice defects and crystallite imperfections.
The anisotropy of the graphite crystal leads to different physical properties and chemical reactivity in different crystallographic directions. The energy of the prismatic plane amounts
As it was shown by Laine and co-workers , the different reactivity of carbon materials can be ascribed to the fact that different carbons have, initially, different amounts of active surface area. Graphite materials with large crystals and few defects have the best chemical stability.
Figure 1. The crystal structure of hexagonal graphite
B.1.2. Chemical reactions of carbon
B.1.2.1. Gas-phase reactions
At room temperature graphite does not react with gases like O2, CO2, H2O and H2. Above
400°C these gases start reacting with graphite. The temperature at which reaction takes place depends on the perfection of the graphite’s crystal structure.
Heterogeneous reactions involving a porous solid and a gas can be controlled by one or more of three idealised steps:
1. Mass transport of the reacting gas from gas stream to the exterior graphite surface. 2. Mass transport of the reacting gas from the exterior surface to active sites and mass
transport of the products in the opposite direction. 3. Chemical reaction at the active sites.
The variation of reaction rate with temperature for gas-carbon reactions can be divided into three main zones (Figure 2).
In the low-temperature zone I, the reaction is controlled by the chemical reactivity of the solid (step 3). There will be almost no concentration gradient of reacting gases throughout the whole volume of the sample due to the low reaction rate, and this provides uniform access to the entire interior surface of the porous material. For the graphite–oxygenreaction the upper limit for temperature will be 500°C, for the graphite–water steam system 850°C .
In the intermediate-temperature zone (zone II), step 2 becomes important. The diffusion of reactants in pores will influence the oxidation rate of the material. At higher temperatures the concentration gradient of the reacting gas becomes steeper within graphite and the gas
concentration becomes zero at a distance R closer to the surface. The activation energy Ea
reaction this temperature region is characterised by temperatures of 850–1350°C and the graphite–oxygen reaction by 500–900°C.
In the high-temperature zone (>900°C for graphite oxygen and >1250–1400°C for graphite– water steam) – zone III – the concentration of the reacting gas is low at the exterior of the solid and the rate is controlled by step 1. Since bulk gas-transfer processes have low activation energies, the apparent activation energy for gas–carbon reactions in zone III is low.
1/T Ln (r ea ct io n ra te ) I a II b III
Figure 2. Ideal reaction zones in graphite : I – reaction rate is controlled by chemical reactivity of the sample; II – reaction rate is controlled by diffusion in pores; III – reaction rate is controlled by gas transport to the exterior surface of the sample; a and b – transition zones
The reactions occurring in the gas–graphite system are: Reactions with oxygen
C(s)+ O2(g) R CO2(g) ∆H = -394.5 kJ/mol Eq. (1)
C(s) + 1/2O2(g) R CO(g) ∆H = -110.5 kJ/mol Eq. (2)
CO(g) + 1/2O2(g) R CO2(g) ∆H = -283.0 kJ/mol Eq. (3)
Where ∆H is the standard enthalpy of formation at 25°C. The above reactions are exothermic and favoured thermodynamically. But carbon does not readily react with air, so kinetic factors are obviously of importance.
Reaction with carbon dioxide Boudouard reaction:
C(s) + CO2(g) R 2CO ∆H = +172.5 kJ/mol Eq. (4)
The equilibrium can be shifted with increasing CO pressure [5, 6] or in the presence of catalyst.
Reaction with water
C(s) + H2O(g) R CO(g) + H2(g) ∆H = +131.3 kJ/mol Eq. (5)
CO(g)+H2O(g) R CO2(g) + H2(g) ∆H = -213.7 kJ/mol Eq. (6)
The hydrogen and CO2produced can then react with carbon
C + CO2(g) R 2CO(g) ∆H = +172.5 kJ/mol Eq. (4)
C + H2(g) R CH4(g) ∆H = -71.81 kJ/mol Eq. (7)
The presence of hydrogen can shift reaction Eq. (5) left . Reaction with hydrogen
C + H2(g) R CH4(g) ∆H = -71.81 kJ/mol Eq. (7)
The mechanism and kinetics of these reactions are described by Walker .
The approximate relative rates of gas–carbon reactions at 800°C and 0.1 atm are given in Table 1.
Table 1. Approximate relative rates of gas–carbon reactions at 800°C and 0.1 atm pressure
Reaction Relative rate
There are a number of investigations of nuclear graphite reactivity under different oxidation conditions in the literature. Results of the oxidation of HTR-10 nuclear graphite IG-11  exhibited three regimes: 400–600°C with activation energy of 158.56kJ/mol, 600–800°C where the activation energy was 72.05 kJ/mol and a “third-zone” regime above 800°C with very low oxidation energy. A comparison of the reactivity of the two types of graphite used in HTR in oxygen and air at 650–900°C (regime II) leads to the conclusion that there is no difference in the behaviour of matrix graphite (A3-27) and standard graphite V483T during oxidation . In the same time at lower temperature (400°C, regime I), matrix graphite is more reactive with respect to air. For the temperature range of 350–520°C, the activation
energy Eafor A3-3 graphite matrix amounts to 110 kJ/mol .
B.1.2.2. Liquid-phase reactions
Graphite does not react with alkaline solutions. Oxidising acids attack graphite to different degree, depending on the nature and surface area of the material. The reaction with concentrated nitric acid is:
C + 4HNO3o 2H2O + 4NO2+ CO2 Eq. (8)
Depending on the reaction conditions, other products may be formed such as graphitic oxide
(C7H2O4), mellitic acid (C6(CO2H)6) and hydrocyanic acid (HCN). Severe oxidation of black
water-soluble aromatic compounds . Besides HNO3, hydrogen peroxide is used for modification
of the carbon surface in order to increase the number of functional groups . The simplified reaction with boiling sulphuric acid is the following:
C + H2SO4o CO2+ 2H2O + 2SO2 Eq. (9)
Graphite reacts with ozone dissolved in alkaline solutions with the formation of CO2 and
polycarboxylic acids as degradation products [13, 14].
At 50 to 90°C in alkaline and acid solutions graphite is oxidised with hypochlorous acid
HClO forming CO2and Cl-.
Oxidation of coal by aqueous NaOCl yields several products: black base-soluble,
water-soluble acids, light-coloured water-water-soluble acids and CO2[16, 17].
B.1.3. Graphite in reactor core structure
B.1.3.1. Design of AVR core structure
The reactor core of AVR represents a cylindrical vessel made of high-purity graphite of 50cm wall thickness which serves as a reflector  (Figure 3). The graphite brick reflector vessel is enclosed in a 50 cm envelope made from carbon bricks (graphite with higher amounts of impurities), which provides shielding and heat insulation. All this composition is surrounded by a double-walled steel liner. The bottom and top reflector also consist of graphite and carbon bricks.
The reflector of the AVR is made of the graphite quality ARS/AMT produced by Sigri . This graphite is based on needle coke and is densified by extruding, which leads to high anisotropy.
B.1.3.2. Nuclear graphite manufacture
The major processing steps in the manufacture of reflector graphite are summarised in Figure 4. The detailed procedure is described in .
Calcined at 1300°C
Crushed, ground and blended Mixed Cooled Extruded, molded or isostatically pressed Baked at 1000°C Impregnated to densify Graphitised at 2500-2800°C Binder pitch
Raw petroleum or pitch coke
Figure 4. The major processing steps in the production of a conven tional
Polygranular graphite consists of two phases: a filler material and a binder pitch. European nuclear graphites are typically made from a coal-tar pitch-derived coke. The coke is usually calcined at 1300°C before it is crushed and blended. The binder phase is coal-tar pitch. The binder plasticises the filler coke particles so that they can be formed. Commonly used forming processes include extrusion, moulding, and isostatic pressing. The binder phase is carbonised during the subsequent baking operation (~1000°C). Frequently, engineering graphites are pitch-impregnated to densify the carbon artifact, followed by rebaking. The final stage of the manufacturing process is graphitisation (2500–3000°C) during which carbon atoms in the baked material migrate to form the thermodynamically more stable graphite lattice. Nuclear graphites require high chemical purity to minimise neutron adsorption and activation of impurities. Also certain elements catalyse the oxidation of graphite and must be reduced to an acceptable level. This is achieved by selecting very pure cokes, utilising a high graphitisation temperature (>2800°C), or by including a halogen purification stage in the manufacture of the cokes or graphite. All low-boiling point impurities will be removed by graphitisation.
Impurities that remain are those which form carbides or are soluble in graphite. For example, vanadium carbide has a melting point of more than 2800°C; boron carbide melts at 2350°C but also forms a substitutional impurity in the graphite lattice, which is extremely stable.
B.1.4. Graphite fuel elements
The graphitic matrix represents the structural material for the spherical fuel elements of high-temperature reactors (Figure 5). In the inner fuel zone of the elements the matrix serves as a homogeneous envelopment for coated fuel particles. This fuel zone has a diameter of 50 mm and is enclosed in a 5-mm thick fuel-free shell .
Figure 5. Sectional view of a HTR fuel element
The fuel particles (diameter 200–600 Pm) are surrounded by a high-porosity buffer layer to limit the internal pressure from gas production. After the buffer layer they are coated with a high-density pyrocarbon layer (BISO) or with a combination of two pyrocarbon layers with a silicon carbide layer in between (TRISO) to retain radionuclides. In the case of BISO particles, the porous carbon buffer layer is ~ 80Pm thick and the pyrolitic carbon layer ~ 110 Pm thick . In TRISO particles the thickness of the outer and inner pyrocarbon coating layers is ~ 35 and 40 Pm, respectively, silicon carbide ~ 35 Pm and buffer ~ 90 Pm .
B.1.5. Pyrolitic carbon coatings for fuel particles
The development of fuel particles, kernels and coatings processing is described in . Pyrolitic carbon is prepared by the decomposition of a carbonaceous gas over a heated surface. The reaction has been carried out over a wide range of temperatures from 1200 to more than 2000°C. Structure and density of the deposited carbon depend upon the deposition mechanism and deposition conditions. The structure of pyrocarbon deposited in a fluidised bed depends mainly on the pyrolysis gas used, i.e. methane, propane, etc., its concentration, the gas pressure, the carrier gas velocity, the surface temperature, substrate geometry and
For example, by methane pyrolysis as a function of temperature and methane concentration three regions with different PyC structure can be distinguished (Figure 6).
Figure 6. Correlation between pyrocarbon structure, density, BAF and deposition conditions of methane 
It is known that isotropic pyrocarbon has the best neutron-irradiation resistance. So the Bacon anisotropy factor (BAF) should amount to 1.0–1.05. The pyrocarbon density that showed the
best properties due to the nuclear reactor conditions ranges from 1.75 to 1.95 g/cm3.
From methane deposition, as can be seen in Figure 6, isotropic carbon with such properties can be obtained at temperatures of 1800–2000°C and methane concentration should be in the range 20–25 vol. %. Pyrocarbon precipitation in the range of higher methane concentration can lead to formation of sufficient amounts of soot to cause a reduction of pyrocarbon density. Operation at this temperature region of pyrocarbon deposition is not favourable because it is difficult to completely prevent uranium and thorium diffusion in the inner pyrocarbon layer during the coating procedure. Therefore, in the German process of coated particle production the outer and inner pyrocarbon layers of TRISO particles are deposited from a mixture of acetylene, propylene and argon at a temperature of 1300°C .
Figure 7. Correlation between pyrocarbon structure, density, BAF and deposition conditions of propylene 
Figure 7 shows he dependence of carbon density, structure and BAF on deposition temperature and propylene concentration. In this case, isotropic carbon suitable for application in nuclear reactor is formed in the temperature region of 1200–1350°C. The crystallite size of this pyrolitic carbon amounts to 20 from 60Å depending on propylene concentrations and fluidised-bed geometry. Pyrolitic graphite has several distinct properties that set it apart from nuclear graphite. They are listed in Table 2.
Table 2. Properties of pyrolitic carbon and nuclear graphite
Properties at room temperature Nuclear graphite Isotropic pyrolitic carbon
Density, g/cm3 1.6-1.81 1.55-2.0
B.1.6. Fabrication method of graphite matrix
Several graphitic matrix varieties were developed . In AVR and THTR reactors standard A3-3 and A3-27 matrixes for spherical fuel elements were used. Both materials are based on the same filler components – natural graphite and artificial graphite – and are of similar composition. The essential difference lies in the binder and its processing. For the A3-3 matrix phenolic resin binder is produced from phenol and formaldehyde. The resin is thermoplastic with a two-dimensional cross-linking. The formation of an infusible, hard solid occurs only after heating to 250°C. In contrast, the binder which is synthesised from the raw materials phenol and hexamethylentetramine for the A3-27 matrix is duroplastic with a three-dimensional cross-linking, and hardening of the binder occurs at temperatures >140°C.
The method for fabricating spherical fuel elements was developed and standardized by HOBEG. The process consists of three main steps:
x preparation of the raw material mixture x moulding of the fuel-free or fuelled spheres x heat treatment of the spheres
The schema of matrix sphere manufacture is shown in Figure 8. The pre-mixed filler components natural graphite and petroleum coke graphite are kneaded with the dissolved phenolic resin binder, dried and ground in a hammer mill.
For the fabrication of fuel elements, the coated fuel particles are coated with resinated powder prior to processing in a rotating drum, in order to avoid damage due to pressing.
The quasi-isostatic cold-moulding operation, in which dies made of silicon rubber are used, consists of two steps:
1. premoulding of the fuelled zone of the sphere at a low moulding pressure of
2. final moulding of the sphere at a moulding pressure of 30 kN/cm2 after the fuelled
zone has been embedded in resinated powder for the sphere shell
Moulding is followed by mechanical machining of the spheres - lathing to specified size. This is followed by a two-stage heat treatment consisting of carbonisation at 800°C and residual degasification at 1800°C and at 1950°C for A3-3 matrix and only at 1950°C for A3-27 matrix.
13 8. HO BE G m et ho d fo r m anu fa ct ur in g sph er ic al fu el el em en ts
B.2. Graphite waste management
B.2.1. Nature of radionuclide contamination
Radioactivity in graphite and carbon/slag results from the neutron capture reaction on carbon itself and on impurities like cobalt, iron, lithium, nitrogen, etc. In the case of AVR, the impurity concentrations in reflector graphite and insulation layers of carbon bricks are different (Table 3). The other contributions to the total inventory of radionuclides in the graphite must also be considered. Besides the activation of carbon and of stable impurities in the graphite these are the fission of natural uranium present in the graphite as an impurity and the possibility of primarily surface contamination from the other regions of the reactor.
Table 3. Concentrations of impurities in AVR graphite
Isolation carbon Reflector graphite
30 2 3H 10 2 3H 990 000 1 000 000 14C 4 500 30 14C 15 0.2 36Cl 1 600 30 40K 1 500 100 41Ca 7 000 1 000 55Fe 10 0.2 60Co 40 10 63Ni 2.5 0.05 94Nb 10 2 93Mo, 99Tc 1 0.01 134Cs 100 20 133Ba 2 0.02 151Sm, 155Eu 0.1 0.02 152Eu, 154Eu Concentration, ppm Tritium
The radionuclide 3H, tritium has a half-life of 12.3 years. The contribution of radioactivity in
nuclear graphite arising from tritium is significant [26-28]. It is produced by the following reactions:
– fission reaction, such as 235U(n,f) 3H reactions,
–6Li(n,D) 3H reactions, lithium is present as an impurity in the graphite matrix of the fuel
element and in the reflector,
– 3He (n,p) 3H reactions of the 3He isotope present in the helium coolant,
Main contribution to accumulation of tritium in graphite is given by neutron reactions with 6Li
and 3He nuclei. Tritium generated from lithium impurities present in graphite is mostly
produced in the graphite bulk. The release of tritium is controlled by its diffusion out of the grain boundaries and into the pore system.
The chemical properties of tritium are essentially the same as those of ordinary hydrogen. One of the most important reactions is isotopic exchange where tritium can replace hydrogen atoms in water molecules or in organic molecules. The exchange process Eq. (10) is rather slow at room temperature (equilibrium constant K=6 at 25°C) because the hydrogen is tightly bound.
HT+ H2O R HTO + H2 Eq. (10)
Radionuclide 14C has a half-life of 5730 years. It is mainly produced in the reactor graphite
through the following neutron reactions:
Table 4. Activation reactions producing 14C
Reaction Capture cross section in barns (10-24cm2) Abundance of isotope in %
13C (n, J) 14C 0.9·10-3 1.1 13C/carbon
14N (n, p) 14C 1.81 99.63 14N/nitrogen
17O (n, D) 14C 0.235 0.04 17O/oxygen
In the reactor core materials nitrogen is present only as an impurity, whereas carbon and oxygen are in some cases major constituent elements of the coolant, moderator or fuel. In
spite of this fact, the 14N activation reaction is usually the most important contributor to 14C
production because of its larger cross section and high isotopic abundance of 14N in natural
nitrogen. Nitrogen in graphite is in the bound state, substituting for carbon atoms in the nodes
of crystal lattice, or in a gaseous form filling pores in graphite. The kinetic energy of the 14C
atom formed is about 470 kJ/mol. This value is equivalent to the bond energy between C–C
bound and C=C bond. It was suggested  that the 14C atom formed stays in the same
position as 14N. Thus the level and location of nitrogen impurity in all reactor core materials is
an important parameter. The nitrogen levels vary widely from 10 to 100 ppm in different reactor graphites  and sometimes they are not known very precisely. It was shown that the nitrogen content is the largest on the surface . From the surface to a depth of about 30 nm, the nitrogen concentration decreases.
The three radioactive caesium isotopes 134Cs, 135Cs and 137Cs are produced by nuclear fission
and neutron capture reactions:
235U o137Cs, 135Cs
235U o133Cs (n, J) 134Cs
134Cs can be also produced from the stable isotope impurity during reaction:
present in the circuit from fuel elements externally contaminated during manufacture, volatilisation of Cs from defect fuel due to its high vapour pressure. This Cs can be absorbed in graphite and form the interstitial compounds .
152Eu, 154Eu, 155Eu are produced by fission reaction and their half-lives amount to 12.4 years,
8.5 years and 4.5 years respectively. The isotopes can be also formed by activation of the
impurities 151Eu,153Eu and 154Sm.
60Co originates from neutron activation of stable 59Co, which is present as an impurity in
nuclear reactor graphite, and has a half-life of 5.3 years.
Table 5 shows the calculated total radioactivity in AVR graphite at the end of 1988 . Table 5. Total radioactivity in AVR graphite
Reflector graphite Isolation carbon
3H 8.8E+14 6.9E+15 14C 4.6E+12 2.9E+14 36Cl 1.5E+09 5.9E+10 41Ca 5.8E+10 4.5E+11 55Fe 1.1E+15 4.0E+15 60Co 4.2E+13 1.1E+15 63Ni 4.1E+12 8.5E+12 93Mo 2.5E+08 4.1E+08 99Tc 2.8E+07 3.5E+07 134Cs 8.9E+11 3.1E+13 133Ba 3.5E+11 7.1E+11 151Sm, 4.5E+08 1.8E+10 152Eu 1.4E+07 2.9E+07 154Eu 1.5E+11 3.0E+11 155Eu 6.3E+10 2.5E+12 166mHo 2.2E+09 4.3E+10 Total radioactivity, Bq
B.2.2. Diffusion of radionuclides in graphite
Diffusion can be defined as the mechanism by which matter is transported into or through matter.
In polycrystalline materials the mechanism of diffusion is very complex. Different types of diffusion are distinguished upon the kind of the medium, and differ in the progressive motion of the atoms and in the rate of diffusion. Volume diffusion describes progressive movement of atoms in a solid with regular lattice structure. The movement of atoms in crystals is possible
mainly due to the presence of different kinds of defects. Different motion possibilities exist for the lattice’s own atoms as well as for foreign atoms  (Figure 9):
a) when an atom is displaced from the lattice site and jumps to neighbouring vacancies or interstitial position.
b) when there is an exchange of lattice positions involving two, three or four atoms situated next to one another in the crystal structure.
Figure 9. Atom movement in crystal lattice: a) jump to neighbouring vacancies or interstitial position, b) exchange of atoms
The other type of diffusion connected with structure of solid substance is grain boundary diffusion. An illustration of the porous structure of graphite is shown in Figure 10. It consists of granules of around a few microns in size with voids in between. The granules themselves are made up of small crystallites. The volume diffusion takes place inside these granules. The demarcation of grains from each other leads to free space, which together with grain surfaces is included in the term the “grain boundaries”. The rate of diffusion along grain boundaries is much faster than that of diffusion in the bulk crystal.
Pore diffusion plays a role in porous materials. If the diffusing atoms form a bond with the grain surface, the mechanism of grain boundary diffusion will be valid. In the case of noble gases (Kr, Xe), when there is no chemical interaction with the surface of material, an unhindered transition of fission gases occurs from grains to pores. Then a free movement of the diffusing atoms is possible as in a gas. Therefore pore diffusion can be compared with the diffusion in gas phase.
The behaviour of radionuclides in graphite at high temperatures is of great importance. It depends on the properties of the diffusing substance. The temperature dependence of the diffusion coefficient is expressed by the Arrhenius equation:
Figure 10. The porous structure of graphite
Reduced diffusion coefficient D’ (s-1) is defined as the diffusion coefficient D (m2/s) divided
by the squared “equivalent sphere” diffusion radius, a (m):
´ D D
a Eq. (12)
The self-diffusion in graphite becomes essential above 2150°C. The diffusion coefficient at
2200°C was determined to be in the range 6.4·10-16 to 3·10-15cm2/s for different types of
nuclear graphite .
Studies of the release behaviour of different radionuclides from graphite have been made. Diffusion coefficient for strontium in LTI pyrocarbon (low temperature isotropic) varies from
10-12 to 10-8 cm2/s in the temperature range 300–730°C. In graphite strontium diffusion is
faster – diffusion coefficient amounts to 10-11–10-6cm2/s for the same temperature .
Caesium release from BISO coated particles is 32% after 1 hour of post-irradiation annealing at 2300°C, and europium release 23% after 3 hours . In the pyrocarbon layer, the caesium
diffusion coefficient was 4·10-11–3·10-8 cm2/s at temperatures of 1600–2200°C.
The experiments with irradiated BISO particles (FIMA 14%) showed that Sr and Cs were released almost quantitatively at 2000°C after 5 hours. 72% of the caesium was released and 26 % was retained in the pyrocarbon layer. The release of Sr was about 92% .
Caesium is a very mobile element. During the procedure of graphite burning Cs can be released from the graphite matrix, volatilised (Cs vapour pressure is 0.1 atm at 750°C) and transported from the furnace into the off-gas [26, 38]. The loss of Cs from graphite due to vaporisation was 15 % of the total amount at 750°C after 9 hours of annealing . The vaporisation of Sr and Ba from the graphite body starts above 1200°C . From 200 °C to 1200°C, atoms of Ba move inside the graphite to active sites and can be leached out later. Tritium emission from Windscale Pile I graphite was studied by Wörner et.al. . After 30 min at 700 °C about 3% of the tritium was released.
Tritium behaviour in reactor graphite is discussed by Fischer and Malka [41, 42]. The reduced diffusion coefficient of tritium from pitch coke AS1-500, petroleum coke AL2-500 and graphite matrix A3-3 was determined (Table 6). The experiments were performed after irradiation of graphite in FRJ-1 (AS1-500 and A3-3) and AVR (AL2-500). In the first case, the temperature during irradiation did not exceed 100°C (cold irradiation). In the case of AVR the irradiation temperature was about 500°C.
The diffusion process of tritium depends strongly on the nature of the graphite samples [43, 44]. As was shown  the release behaviour depends strongly on the extent of graphite anisotropy and the diffusion of tritium in isotropic graphite will be faster than in anisotropic graphite.
Table 6. Diffusion coefficients of nuclear graphite
Type of graphite Temperature, °C Diffusion coefficient, D' s-1
A31) 800 1.72E-09 A31) 850 9.09E-09 A31) 900 6.89E-08 A32) 1000 8.18E-09 AS1-5002) 1050 9.83E-11 AL2-5002) 1025 1.83E-10 1) - , 2) - 
B.2.3. Options of graphite waste management
The management options considered for graphite waste [28, 45] are as follows: x disposal on the deep ocean bed
x shallow land burial x incineration
x deep geological disposal (inland site and coastal site) Ocean-bed disposal
Disposal of graphite on the deep ocean bed would lead to a slow release of activity into bottom waters by leaching, and gradual dispersal throughout the world’s oceans. The main
contribution to collective doses would be the global circulation of 14C.
Shallow land burial
The shallow land burial facility is assumed to be a fully engineered concrete structure incorporating barriers against infiltration of groundwater, and located in a clay formation with relatively low groundwater flow. The possibility of long-term leaching of activity from the graphite by groundwater, followed by movement to the soil zone and into crops and drinking
This option for graphite processing enables the volume of radioactive wastes to be reduced.
However, CO2 formed leads to the release of 14C into the atmosphere. 14CO2 penetrates into
the metabolism of the plant and animal world by photosynthesis. Because of its long half-life
and the biological significance of carbon, the release of 14C from nuclear facilities could have
a major radiological impact on the environment and mankind. Deep geological disposal
Two different types of deep geological disposal were considered. The first is an inland site in different rock units, which could lead to very long transit times for radioactivity transported by moving groundwater. The second – a coastal repository – is assumed to be sited in shale. Here water movement can be relatively fast and the risk of radionuclides transport to biosphere will be also higher.
In the frame of the present work the graphite incineration and storage in deep geological formation will be viewed in more detail in Chapter B.2.4 and Chapter B.2.5.
B.2.4. Reprocessing of contaminated graphite
In the context of the final disposal route it is important to reduce waste volume. Processing of graphite by incineration offers the opportunity to separate the major fraction of the graphite mass from the short-lived radioisotopes . Only small residues (ash) remain for final
storage. However, the release of 14C into the atmosphere accompanied by graphite burning is
J.B. Mason and D. Bradbury  suggested burning waste graphite without CO2 release into
environment. This methodology involves the use of pyrolysis/water steam reforming followed by off-gas control. The exhaust gas can be solidified in the form of calcium carbonate, which could be used to fill voids in other radioactive waste packages. It was suggested that the process could either be used to process graphite removed from the core or even applied to gasify graphite waste within the core.
Two options have been considered for the conversion of carbon dioxide to an alkaline earth carbonate . The first is direct precipitation:
M(OH)2+ CO2o MCO3+ H2O Eq. (13)
(M = Ca, Sr or Ba).
The second alternative is the double alkali process. In the first step, carbon dioxide is adsorbed by sodium hydroxide solution. The resulting sodium carbonate then reacts with an alkaline earth hydroxide in a separate vessel to precipitate the carbonate and regenerate sodium hydroxide for recycling:
2 NaOH + CO2o Na2CO3+ H2O Eq. (14)
Na2CO3+ M(OH)2o 2 NaOH + MCO3 Eq. (15)
However, reprecipitation of carbon dioxide in carbonate form does not solve the problem of volume waste reduction. Moreover, carbonate wastes are less stable to leaching than graphite
in elementary form. The dissolution rate of CaCO3 reported in  amounts to
5.94·10-7mol/(cm2·d). For MgCO
and ~10-9 mol/(cm2·d) in the pH range 5–8 . Whereas the graphite oxidation rate in pure
water was determined as ~10-11mol/(cm2·d) .
Figure 11. Graphite treatment scheme
Carbon from the gas phase can be precipitated in the form of elementary carbon as likely to be resistant to leaching. Contaminated graphite reacts with water steam in a fluidised bed with the formation of CO. Elementary carbon can be obtained from carbon monoxide by the Boudourd reaction:
2 CO R C + CO2 Eq. (4)
This reaction is exothermic from left to right. High conversion of carbon monoxide to carbon is possible at a relatively low temperature in the presence of a catalyst [52, 53]. The problem is that only half of the carbon reacting will be immobilised as a solid. The other half (as carbon dioxide) would have to be recycled. The preferred procedure in this case is gasification
of graphite with H2 in order to form methane. Subsequent pyrolysis of methane yields
elementary carbon in the form of soot.
B.2.5. Deep geological disposal
B.2.5.1. Host rock types
For the purpose of waste disposal in geological formation three types of rocks (argillaceous or “clay-rich” units, hard crystalline igneous and metamorphic rocks, and evaporites – halite formation) are considered as host units. All of them have a low permeability and therefore low rates of water through-flow in terms of volume and velocity.
Hard stable crystalline rocks (granite, gabbro and basalt) have low total porosity. However they are generally joined and fractured. Water flow through the rock is dominated and controlled by these fissures. Therefore crystalline rocks can be considered more or less permeable, although the contribution of the fracture to the porosity of these rocks is small. Argillaceous rocks, although they differ in physical properties, ranging from plastic clays to hard, well-bedded and often fractured units, are characterised by low permeability and high sorption capacity (radionuclide retardation potential).
Evaporite (salt) deposits were thought to be completely impermeable and they also have the additional advantage of being plastic enough to allow self-sealing of fractures by creep in response to heat and stress. Evaporites are units of soluble salts of Na, Mg, K and Ca formed in the geological past by evaporation of shallow lagoons and lakes in cyclic episodes. Chlorides, sulphates and carbonates may be laid down in layers with various degrees of mixing of salts. The most common salt is halite rock salt, NaCl. So the composition of corrosive groundwaters will be determined by the chemistry of salt with which they interact. For heat-generating radioactive waste forms, salt rock, for example such as Gorleben salt dome [54, 55], is considered to be a good host medium because of the unique viscoplastic properties which, with lithostatic pressure plus temperature as the driving forces, will build up a natural barrier within a few years after emplacement of the waste packaging.
B.2.5.2. Multi-barrier system
Conservative assumptions on scenarios for post-operational period are made for the long-term safety considerations. It is presumed that water can penetrate into the repository due to consequences of engineering and waste replacement. Water intrusion may produce a harmful effect on the integrity of the waste forms and in the course of time lead to mobilisation of radionuclides.
The repository design should ensure long-term isolation of the waste and thus comprise a system of geological and engineered barriers to prevent the release of the waste from the packages and the movement of radionuclides to biosphere. The multi-barrier system includes four components (Figure 12).
The first is the waste form itself, which immobilises the waste radionuclides in a solid matrix. In the case of HTR fuel element it has its own subsystem of protective layers: graphite matrix, dense pyrocarbon coating, silicon carbide layer, porous pyrocarbon coating (buffer), and fuel in the form of the stable leach resistant ceramic.
The second barrier is the metallic canister in which the waste will be sealed. To minimise water movement around the container and to ensure that the waste block is in mechanical and thermal continuity with the rock, it is necessary to fill the emplacement hole with some backfill material – third barrier. The back-fill material should also possess a good adsorptive activity towards the radionuclides, which may be leached from the waste package. The waste matrix, container and back-fill material are termed the “engineered barriers”.
Figure 12. Migration and immobilisation of radionuclides in the multibarrier system The final barrier is the host rock and geological environment (geological barrier) in which the repository is constructed.
B.2.5.3. Water radiolysis in repository
In a final repository an aqueous phase, which may migrate towards the radioactive waste package, will be irradiated by spent fuel elements. The radiolysis of water produces both molecular and radical oxidants and reductants , which may influence the redox conditions in the repository and the stability of the waste form, container and buffer materials.
Radiolysis of pure water
The radiation chemistry of water and aqueous solutions is usually described in terms of the spur diffusion model.
Several pairs of radicals or ions (primarily e
-aq, OH· and H3O+in pure water) are formed in
small isolated volume elements (spurs) in the initial radiation process. Species within the spurs interact as they diffuse into homogeneous distribution and these interactions result in the reformation of water and in the formation of molecular products. In pure water under
J-irradiation the decomposition products which appear in homogeneous distribution are e
The overall process of radiolysis is usually divided into three stages.
The physical stage consists of energy transfer to the system. Its duration is of the order of
10-15sec or less. Ionisation or excitation of water takes place
H2O + irradiation o e-+ H2O+ Eq. (16)
The physicochemical stage consists of processes, which lead to the establishment of thermal
equilibrium in the system. Its duration is of the order of 10-11 sec or less. Electrons ejected in
the ionisation process become thermolised and hydrated:
-therm o e-aq Eq. (18)
The H2O+ions undergo a proton transfer reaction with neighbouring water molecules:
H2O++ H2O o H3O++ OH· Eq. (19)
and the H3O+becomes hydrated.
The dissociation of excited water molecules gives the hydrogen atom and hydroxyl radical as main products
H2O*o H· + OH· Eq. (20)
It also gives a low yield of hydrated electrons and, eventually, molecular hydrogen. The contribution of excited water molecules to the formation of primary free-radical products in water radiolysis is of minor importance in comparison with that of the ionisation processes. The chemical stage consists of diffusion away from the point of origin and chemical reaction
of primary species (e
-aq, OH·, H3O+ and H), and leads to the establishment of chemical
equilibrium. It begins in the spur about 10-11 sec after the passage of the radiation and about
10-10 sec in the bulk of the solution. The radiation-chemical yield of primary species G is
determined as the number of species produced or disappearing per 100 eV of energy absorbed. Molecular hydrogen is formed from recombination:
2H2O e -aq+ e-aq o H2+ 2OH- Eq. (21) H2O e -aq+ H·o H2+ OH- Eq. (22) H· + H· o H2 Eq. (23)
The first reaction is the most important.
Atomic hydrogen arises primarily from Eq. (20) and reaction Eq. (24):
-aq+ H3O+o H· + H2O Eq. (24)
The recombination of hydroxyl radicals is the way to give hydrogen peroxide as the final product.
OH· + OH· o H2O2 Eq. (25)
Important water reformation reactions are
e -aq+ H2O2o OH· + OH- Eq. (26) e -aq + OH· o OH- Eq. (27) OH-+ H 3O+o 2H2O Eq. (28)
The principal radiolytic products in pure water or dilute aqueous solutions are listed in Table 7.
Table 7. Primary products in irradiated water
Irradiation H2 H· e
-aq H2O2 OH· HO2· H+
J 0.43 0.61 2.7 0.61 2.86 0.03 2.7
D 1.4 0.3 0.3 1.3 0.5 0.1 0.3
G-Values (molecules per 100 eV)
Radiolysis of salt brines
Reactive solutes at high concentrations can react with radicals and thus change G-values from those in pure water and cause the formation of additional G-species.
In concentrated neutral chloride solution OH radicals will be removed by the reaction Eq. (29) :
OH· + Cl-+ H
3O+o Cl· + 2H2O K = 1.7x1010 Eq. (29)
In acid solution this reaction will be also of significance. It will cause a reduction of OH· and
H2O2 production from that in pure water and will promote the increase of e-aq and H2. High
hydrogen production has been observed in the J- and D-radiolysis of brines . Also chlorate, hypochlorite and chlorite can be formed as stable products . Formation of hypochlorite can be related to the chain of reactions, which take place during J-irradiation of chloride solutions: Cl-+ Cl· oCl 2- K = 2.1x1010 Eq. (30) Cl2-+ Cl2- o Cl3-+ Cl- K = 7x10-9 Eq. (31) Cl3-o Cl2+ Cl- K = 5x104 Eq. (32) Cl2+ H2O o Cl-+ H++ HClO Eq. (33)
Chlorate can be formed from Cl2 through reactions involving radicals; it can be formed from
2-+ Cl- Eq. (34)
ClO2-+ ClO-o ClO3+ Cl- Eq. (35)
The radiation chemical reactions occurring in the presence of Cl- ions were published by
Sunder . The formation of different chlorine oxidising species is associated with a high redox potential which can reach 1200 mV [45, 60]. Under such conditions the behaviour of protective barriers can differ from those in the absence of J-irradiation.
C. Experimental part
The following technical equipment was used:
Drying oven Heraeus T-12
Gas chromatograph 1: SiChromat 2 from Siemens
separating columns: Porapak QS (80/100 mesh, L=1 m, ID=2mm) and molecular sieve 5 Å (80/100 mesh, L=2x3 m, ID=2 mm)
carrier gas: argon
2: SiChromat 2 from Siemens
separating columns: Poraplot Q (L=10m, ID=0.32mm) and molecular sieve 5 Å (25 m, ID=0.32mm)
carrier gas: helium
Optical microscope Karl Zeiss KS300 with image processing software
Scanning electron microscope Jeol JSM 840 coupled with EDX unit Tracor
(SEM) Northerm 5502
Furnace combustion furnace C-5500 from Ströhlein Instruments;
tube furnace, adjustable up to 1550°C
BET surface area measurements Junior Quantosorb, QUANTOCHROM
Balance MP-3000, YMC Europe GmbH
Liquid scintillation counting (LSC) TRICARB 2100, Packard
CO, CO2 analyser NGA 2000 MLT analyser from Fisher-Rosemount,
concentration range 0–4000 ppm
Flow controller mass flow controller 5850E, Brooks
range: 0–80 L/h
J-spectrometer High-Purity Germanium Well Detector from EG&G
X-ray diffraction (XRD) Stoe Stadi transmission diffractometer coupled to a
Cu-anode X-ray tube and using CuKα radiation with λ = 1.5406 Å at 40 kV and 30 mA
Water purification Elga Elgastat maxima HPLC
C.2. Reagents and materials investigated
The following chemicals were used:
MgCl2·6H2O CaCl2·2H2O NaCl KCl K2SO4 NaOH MgSO4·7H2O CuO HCl HNO3 H2O2
All chemicals were from MERCK, Darmstadt, and of analytical grade. They were used without preliminary treatment.
Graphite matrix A3-3: graphite powder
Pyrocarbon: coatings from unirradiated BISO fuel particles, intact
BISO and TRISO particles (dimensional characteristics are listed in Table 33, appendix)
Merlin reactor graphite: bottom right channel of thermal column II
AVR graphite: inner reflector
Argon: purity >99.999%, MESSER Grisheim
Oxygen: purity >99.5%, LINDE
Calibration gas: mixture CO – 1880 vpm, CO2 – 2180 vpm,
O2– 0.516 vol%, H2– 4 vol%, N2 – rest;
MESSER Grisheim Preparations of brines
Brine-2. 937.08 g MgCl2·6H2O was mixed with 300 mL of deionised water heated up to 70°C
and stirred until the main part of the magnesium chloride was dissolved. Then 0.126 g
MgSO4·7H2O, 4.13 g NaCl, 1.42 g KCl and 39.68 g CaCl2·2H2O were added. Stirring was
stopped when the solution became clear. After cooling to room temperature, the solution was placed in 1 L volumetric flask and water was added to the filling mark.
Brine-3. 309.4 g NaCl was dissolved in 0.5 L of deionised water and stirred at 70°C up to
complete dissolution. Then 2.74 g CaCl2·2H2O, 2.83 g K2SO4 and 4.0 g MgSO4·7H2O were
added. When the solution was clear it was cooled down and placed in 1L volumetric flask and the water level was brought up to the filling mark.
Table 8. Composition of aqueous phases  NaCl KCl K2SO4 MgCl2 CaCl2 Brine-2 1.49 0.4 – 97.21 5.68 Brine-3 108.65 – 0.67 0.32 0.38 3.61 7.07 Concentration mol/1000mol H2O pH(90°C)
C.3. Performance of experiments
C.3.1. Graphite oxidationC.3.1.1. Sample preparation
Graphite was filed from a dummy fuel element on a turning lathe. The graphite powder was separated by sieving into different fractions with particle size: >0.8 mm, 0.8–0.5 mm, 0.5– 0.25 mm, 0.25–0.15 mm, 0.15–0.05 mm, <0.05 mm.
Pyrocarbon coatings were obtained from disintegration of unirradiated BISO fuel particles. Fuel particles were disintegrated by mechanical cracking in a milling machine. After separation the coatings were additionally milled in mortar.
C.3.1.2. Oxidation experiments without irradiation Two different series of experiments were performed: – long-term experiments
– short-term experiments
Long-term experiments were performed in glass tubes at 90°C under different atmospheres. 1 g of graphite or pyrocarbon was immersed in 50 mL of aqueous phase in a glass vessel with
a total volume of 110 mL. Then the tubes were evacuated, filled with Ar, O2or air and sealed
by melting. The experimental details are summarised in Table 26 (see Appendix).
Short-term experiments were performed with the addition of different concentrations of H2O2
(10-3mol/L, 10-2mol/L, 2.1·10-2 mol/L, 3.2·10-2 mol/L, 5.4·10-2 mol/L, 1.1·10-1mol/L,
1.6·10-1mol/L, 2.7·10-1mol/L) to simulate the radiolysis process. 1 g of graphite powder
fraction <0.05 mm was placed in glass vessels with 20 mL of distilled water and brine-2
solution. Then 30% H2O2 was added in amounts from 2 µL to 500 µL and the system was
evacuated, flushed with argon a few times, finally filled with argon and closed. The experiments with hydrogen peroxide were performed in glass vessels with valves. The volume of the glass vessels was 36 mL.
C.3.2. Oxidation experiments under J-irradiation
Experiments with graphite powder, pyrocarbon coatings and also with intact graphite pieces and intact unirradiated fuel TRISO and BISO particles were performed under J-irradiation in the MTR cooling pool. 1 g of carbon coatings or graphite powder and 10 mL of liquid phase (distilled water, brine-2 or brine-3) was placed in glass vessel with a total volume of 36 mL.
argon and sealed. Sealed vessels were placed in an inner irradiation container (Figure 13). The container was equipped with a heater in order to maintain the temperature at 90°C. It was placed in an outer irradiation container and then in the MTR cooling pool. The irradiation was produced by four spent MTR fuel elements situated along the perimeter of the container. All experimental equipment and the position of container in the cooling pool are shown in Figure 14. The scheme of the irradiation containers with heating system is also presented in Figure 49 in Appendix.
Figure 13. Glass tubes used for experiments in MTR cooling pool (left) and container with glass tubes (right)
MTR fuel elements
Figure 14. a – Outer container, heater, inner containers; b – Position of outer container in MTR cooling pool
The experiments with crushed materials lasted for 6 months. Sampling was performed every two months. The profile of dose rate at the place of container versus time is presented in Figure 15. The integral J-dose over the period of 6 months amounted to approximately 5.3 MGy. In order to provide the same dose rate during the entire period, radiating elements were replaced by a fresh set after 78 days.
With intact material the experiments took about 23 days and the total absorbed dose amounted to ~1 MGy.
All experiments included blanks, which contained only the liquid phase and atmosphere (air, argon or oxygen). 0 0.5 1 1.5 2 2.5 0 50 100 150 200 Time, days D os e ra te , KG y/ h
Fresh spent fuel elements
Figure 15. Dose rate in cooling pool versus time
C.3.2.1. Sampling procedure and calculation of amounts of graphite corroded
The gas phase in the tubes was analysed by gas chromatography. The glass tube was connected to a manometer and a gas mouse. Then the system was evacuated and flushed with argon several times. After final evacuation, the sealing of the vessel was broken by means of an iron ball, which was moved from the outside by a magnet (Figure 50 in Appendix). The gas was trapped in the gas mouse. The established equilibrium pressure after breaking the seal was measured and from this value the pressure in the sealed ampoule was calculated. The scheme of the sampling procedure is shown in Figure 50.
The calculation of reaction rates was performed assuming CO2 equilibrium between aquatic
and gas phases. To attain the equilibrium, the glass vessels were cooled down and maintained at room temperature for 4 hours before sampling.
The amount of CO2in the gas phase Qg(mol) is:
2 0 2 CO g CO g g P V P X V RT RT Q Eq. (36) 0
P – total pressure in glass vessel (atm)
Vg– volume of gas phase in glass vessel (L)
X – fraction of CO2 in the gas phase (vol. %)
R – gas constant – 0.082 (L atm/(mol K)) T – temperature (K)